Synthesis and characterization of ZnO nanostructures using palm olein as biotemplate
© Ramimoghadam et al.; licensee Chemistry Central Ltd. 2013
Received: 25 February 2013
Accepted: 11 April 2013
Published: 20 April 2013
A green approach to synthesize nanomaterials using biotemplates has been subjected to intense research due to several advantages. Palm olein as a biotemplate offers the benefits of eco-friendliness, low-cost and scale-up for large scale production. Therefore, the effect of palm olein on morphology and surface properties of ZnO nanostructures were investigated.
The results indicate that palm olein as a biotemplate can be used to modify the shape and size of ZnO particles synthesized by hydrothermal method. Different morphology including flake-, flower- and three dimensional star-like structures were obtained. FTIR study indicated the reaction between carboxyl group of palm olein and zinc species had taken place. Specific surface area enhanced while no considerable change were observed in optical properties.
Phase-pure ZnO particles were successfully synthesized using palm olein as soft biotemplating agent by hydrothermal method. The physico-chemical properties of the resulting ZnO particles can be tuned using the ratio of palm olein to Zn cation.
KeywordsZinc oxide nanostructures Palm olein Biotemplate Soft templating Palm oil Hydrothermal synthesis ZnO
Nanostructures and nanomaterials are subjected to a research focus in material science due to their unique properties and extensive applications. Among them, ZnO is of a great interest due to its wide band gap (3.37 eV) and large exciton binding energy (60 meV). It has wide applications in different industries including photodetectors , sensors , solar cells , antibacterial for medical products [4–6], cosmetics , etc. ZnO nanostructures can be synthesized by various chemical or physical methods such as precipitation , sol–gel , solvo/hydrothermal , chemical vapor deposition , spray pyrolysis , etc.
In fact, the specific properties of ZnO and its applications depend on its morphology, size and structure. Therefore, lately many researchers are more interested to explore the methods of synthesis of nanomaterials. To meet this requirement and along with developing the common synthesis methods of nanostructures, an increasing surge for utilizing bio-inspired synthesis, has been developed. A green approach for nanomaterials synthesis by applying biotemplate allows the reaction to proceed usually in milder conditions. In addition, due to their ability to form specific structures and self-assembling function, biomolecules may act as templates to synthesize functional nanomaterials of different morphologies. Based on this fact, lots of biomolecule-assisted syntheses of nanomaterials and nanocomposites have been reported recently. Some of them include L-cysteine, lysine [13–16], gelatin  and PEG , to name a few. Additionally, some biotemplates have been used for the synthesis of ZnO nanoparticles namely orange juice , albumen , cyclodextrin , egg-shell membrane , silk , peptide structures , DNA , pollen grain , wood , and different types of microorganisms [28–30]. In principle, the process of biotemplating can be described as seeking to either replicate the morphological characteristics and the functionality of a biological species or the use of biological structure to guide the assembly of inorganic materials , followed by removing of the template and finally forming a pure phase material with the required morphology.
A possible substitute for biotemplate material to mediate the morphologies of inorganic materials is palm olein. Palm olein is the liquid fraction of palm oil which is highly monosaturated and rich in oleic acids . Generally, it contains 46% oleic acid, 37% palmitic acid, 11% linoleic acid, 4% stearic acid and 1% myristic acid. Two major grades of palm olein are produced in Malaysia, standard olein and double fraction (or super) olein . Palm olein application extended from daily usage in the kitchen toward the industrial due to its excellent physical properties and oxidative stability. The use of palm olein to synthesize ZnO nanoparticles offers the benefits of eco-friendliness, low-cost and amenability for large scale production. Moreover, the existence of various functional groups such as hydroxyl and carboxylate should offer a wide variety of nucleation sites for surface controlled inorganic deposition, and could be used in the synthesis of inorganic materials.
Previous works showed palm oil and palm olein have been used extensively as source of carbon  and to produce biodiesel due to its rich sources of fatty acids . There are several studies in which the effect of different fatty acids including oleic acid , ricinoleic acid  were investigated on the formation of nanostructure materials. It is assumed that the carboxyl head group of fatty acid will chemically bound to the surface of nanostructures and modify the surface structural property of particles . To the best of our knowledge, the present study is the first report on ZnO nanoparticles synthesized using palm olein as biotemplate.
Results and discussion
In the case of ZnO samples synthesized using 8 and 16 mL of palm olein (PO) by CVD method, the pure phase of ZnO could not be achieved. Different peaks could be observed from the XRD patterns even after further treatment by two times calcinations at 500°C and 800°C for 5 and 3 hours, respectively. This shows that the pure phase of ZnO with high concentration of PO cannot be achieved through the CVD method under our experimental condidtion. Therefore we continue with the low concentration of PO through hydrothermal method.
Morphology and size
Figure 2e and f images show ZnO sample synthesized at 2 mL PO. The morphology of the ZnO particles has been slightly changed in comparison with that of the ZnO synthesized using 1 mL PO, showing flower-like particles consisting of lots of nano- and micro-sized sheets. A closer look on the as-synthesized ZnO products using 1 and 2 mL PO, reveal that with increasing the concentration of PO, the size of particles increased but the diameter is dramatically decreased. The thin sheets of ZnO crystals assembled like petals of a flower from edge to centre.
FESEM images of ZnO particles synthesized using 3 mL PO are shown in Figure 2g and h. The overall shape of flower-like can be easily seen from the morphology of the particles. However, detailed view on the particles shows that similar structure of three-dimensional star-like particles appears in this sample. It is notable that particles seems to merge together and became embedded with the adjacent particles. Therefore the formation of the structure seems to be incomplete and even sometimes unclear. In addition, very much agglomerated structure can be seen from FESEM images in some areas. Another difference in the morphology of these products that can be taken into account is that corners of the sheets show curvature-like shape for ZnO particles prepared using 3 mL PO while those prepared using 2 mL PO shows that the corners of the sheets are clearly sharp and orthogonal.
ZnO particles prepared using 4 mL PO is shown in Figure 2i and j. Even though the structure of the particles demonstrates the same flower-like shape as seen in Figure 2j, the overall morphology has been changed to some extent. In other words, it contains lots of plate-like particles assembling laterally as petals of a flower while other particles located vertically in the centre.
Generally the mechanism of “biotemplate” can be described either by replicating the morphological characteristics and the functionality of a biological species or using a biological structure to guide the assembly of inorganic materials. In the case of palm olein, which is a complex biomacromolecular, biologically guided assembly of zinc nanostructures has been possibly occurred with the presence of PO functional groups. These functional groups are produced due to the hydrolysis of palm olein in water under the experimental condition stated in the experimental part, created nucleation sites for zinc crystal growth and then promote the pattern or certain morphologies formation. The self-assembly is guided by the presence of the biotemplate and is directed by covalent or non-covalent interactions or molecular recognition process . The electrostatic interaction may occur between carboxyl and hydroxyl groups of PO and zinc cations. This electrostatic attraction may also occur between primary and secondary particles resulted in the formation of complex structures. It is noteworthy that changes in the concentration of PO in the mother liquor, resulted in changing the environment for the nucleation and reaction thermodynamics and subsequently leads to different assemblies for primary and tertiary particles and resulted in different morphologies.
Moreover, this template-assisted method is considered as soft-templating method since palm olein, an organic template, was used to synthesize mesoporous zinc oxide nanostructures. The formation of zinc oxide nanostructures can be summarized in three steps; first - the self-assembly of the palm olein, second - the organization of zinc acetate over the PO self-assembly in regular ordered array to form a stable inorganic-organic hybrid and finally, the successful removal of organic template to get a phase-pure zinc oxide.
Therefore, from particle size results show that ZnO samples synthesized with the presence of palm olein could lead to form both micro- and nanostructures. It is noteworthy that particles as small as 20 nm could be produced when palm olein was used as biotemplate.
To investigate the bio-template effect on the synthesis of ZnO nanoparticles prepared by hydrothermal method, FTIR spectra were measured at room temperature using the KBr pellet technique in the range of 4000–400 cm−1. Samples were gently mixed with 250 mg KBr powder and compressed into discs at a force of 13kN for 5 min using a manual tablet presser.
The characteristic peak of ZnO FTIR spectra are shown in Figure 4b which were recorded separately in the range of 600–280 cm-1. The peaks at about 300–370 cm-1 are in good agreement with the observation of previous work . As seen from Figure 5, ZnO characteristic peaks have shifted to higher wavenumbers from 350–380 cm-1 which is much closer to the absorption peak of commercial ZnO (380 cm-1).
The second weight loss, which can be clearly observed for sample synthesized using 3 and 4 mL PO at about 335°C is assigned to fatty acids decomposition. The percentage of weight loss is 10.0 and 1.4% for sample synthesized at 3 and 4 mL PO, respectively. In the case of samples prepared using 1 and 2 mL PO, peaks are not observed probably due to the presence of a little amount of PO which is still remain in the sample.
The third weight loss occurs at about 410°C is attributed to mono-/diglyceride . This step includes 0.6, 1.2 and 0.8% weight loss percentages for samples synthesized at 2, 3 and 4 mL PO, respectively. As seen from Figure 6a, DTG curve shows very weak peak at this temperature for the sample synthesized at 1 mL PO.
Finally, the last weight loss of 1% at 634°C is due to dehydroxylation of residual palm olein. This step has been shifted to higher temperature, 970°C, for the sample synthesized at 3 mL PO which can be due to the high heating rate. However, it can be easily interpreted from the curve that the degradation has not been leveled off possibly even after 1000°C. Therefore, the high percentage of 25% weight loss demonstrates that sample prepared at 3 mL PO adsorbed the highest amount of palm olein which is in good agreement with the FTIR results. It should be noted that high heating rate of 10°/min is resulted in overlapping, shifting or even disappearing of the peaks as mentioned earlier.
The desorption branch of isotherms are quite similar, due to similarity in their pore’s texture, though the ZnO sample synthesized at 3 mL PO shows a different desorption branch. The adsorption-desorption isotherm of sample synthesized using 3 mL PO indicates that the evaporation of the condensed liquid from pores is delayed. Therefore, the access of adjacent pores to the vapor phase can be achieved instead . As a result, the desorption branch does not follow the original hysteresis loop.
More uniform pores can be observed for the ZnO samples prepared using PO compared to the one synthesized without PO. The ZnO samples synthesized using 1 and 2 mL PO show higher pore volume in smaller pore range (2–20 nm) and lower pore volumes with bigger pore range (20–70 nm), respectively compared to the sample prepared without PO. The pore size distribution for sample synthesized at 3 mL PO is shown in Figure 8 (inset). A dual mesoporous distribution at 14 and 46 nm can be clearly seen. The overall shape of the size distribution for the sample prepared using 3 mL PO is different from the others indicating different pore texture. Moreover, in the case of ZnO synthesized using 4 mL PO, a narrowest pore size distribution was observed which demonstrates the formation of more uniform pores.
All chemicals used in this work were of analytical reagent grade and used as received without any further purification. All the aqueous solutions were prepared using deionized water. Palm Olein (PO) was purchased from a market in Malaysia.
In a typical procedure, 1 g of zinc acetate (Zn(Ac)2.2H2O) and 0.8 g sodium hydroxide (NaOH) were dissolved in 25 mL distilled water under constant stirring (Zn2+ : OH- = 1: 4). The measured pH was 13. After 1 hour stirring, different volumes of palm olein, 0, 1, 2, 3, 4, 8 and 16 mL were introduced to the solution (i.e. the ratio of zinc acetate to palm olein was 1:0, 1:1, 1:2, 1:3, 1:4, 1:8 and 1:16, w/v%) and stirring was continued until palm olein was completely dissolved, i.e. a flocculent precipitate rather white in color was obtained. Finally, the mentioned solution was transferred into a Teflon-lined stainless steel autoclave, 50 mL and hydrothermal growth was carried out at 120°C for 18 h. After treatment, the autoclaves were allowed to cool down and the precipitates were collected, centrifuged and the supernatant was discarded. The obtained particles were washed three times with ethanol and distilled water, in order to remove impurities and dried at 60°C for 24 h.
Samples with high concentrations of palm olein (8 and 16 ml PO) were not able to dry at 60°C even after several days. The solutions were oily and sticky. Therefore we changed the hydrothermal method to chemical vapor deposition (CVD). After preparing the solution as discussed earlier, the yellowish solution was transferred into ceramic boat. Then the boat was placed at the center of the furnace’s tube. The process of heating was performed for 2 hours at 500°C under N2 gas atmosphere. Then samples were allowed to cool down and the precipitates were collected and ground to powder form.
Powder X-ray diffraction (PXRD) analysis was performed on a Shimadzu diffractometer, XRD-6000 (Tokyo, Japan) equipped with CuKα radiation. The morphology of the micro- and nanostructures were characterized by a field emission scanning electron microscopy (FESEM) a JOEL JSM-6400 (Tokyo, Japan). Particles Size distribution was analyzed by a Malvern zetasizer nano series ZEN1600 (Worcestershire, UK). Fourier transform infrared spectra were recorded over the 280–4000 cm−1 range using a Perkin-Elmer 100 spectrophotometer (Waltham, MA, USA) under standard conditions. Thermogravimetric and differential thermogravimetric analyzer were carried out using a Mettler Toledo instrument (Greifensee, Switzerland) using heating rate of 10°C/min, in the range of 25–1000°C under nitrogen atmosphere. Surface characterization of the material was carried out using nitrogen gas adsorption-desorption technique at 77 K by a Micromeritics ASAP 2000 (Norcross, GA, USA). The UV-VIS-NIR spectrophotometer UV-3600 SHIMADZU was used to determine the optical properties.
Pure phase ZnO particles were successfully synthesized using palm olein as soft biotemplating agent, which lead to form both micro- and nano-structure particles. Different morphologies, namely flower-, flake- and star-like particles could be obtained. The morphology changes can be possibly due to the reaction between carboxylic group of palm olein and zinc hydroxide groups, which has been physically occurred on the particle surface. Moreover, maximum weight loss of approximately 25% was observed due to the template degradation. In addition, biotemplate could be also used to modify the surface properties of ZnO particles.
The authors are gratefully acknowledged the Ministry of Higher Education of Malaysia (MOHE) for financial support under grant No. FRGS/1/11/SG/UPM/01/2 (Vot No. 5524165).
- Liang S, Sheng H, Liu Y, Huo Z, Lu Y, Shen H: “ZnO Schottky ultraviolet photodetectors”. J Cryst Growth. 2001, 225 (no. 2–4): 110-113.View ArticleGoogle Scholar
- Lin Y, Zhang Z, Tang Z, Yuan F, Li J: Characterisation of ZnO-based Varistors Prepared from Nanometre Precursor Powders. Adv. Mater. Opt. Electron. 1999, 9: 205-209. 10.1002/1099-0712(199909/10)9:5<205::AID-AMO383>3.0.CO;2-8.View ArticleGoogle Scholar
- Golego N, Studenikin SA, Cocivera M: “Sensor Photoresponse of Thin-Film Oxides of Zinc and Titanium to Oxygen Gas”. J Electrochem Soc. 2000, 147: 1592-10.1149/1.1393400.View ArticleGoogle Scholar
- Sawai J: Quantitative evaluation of antibacterial activities of metallic oxide powders (ZnO, MgO and CaO) by conductimetric assay. J Microbiol Methods. 2003, 54 (2): 177-182. 10.1016/S0167-7012(03)00037-X.View ArticleGoogle Scholar
- Zhang L, Jiang Y, Ding Y, Povey M, York D: Investigation into the antibacterial behaviour of suspensions of ZnO nanoparticles (ZnO nanofluids). Journal of Nanoparticle Research. 2006, 9 (3): 479-489.View ArticleGoogle Scholar
- Raghupathi KR, Koodali RT, Manna AC: Size-dependent bacterial growth inhibition and mechanism of antibacterial activity of zinc oxide nanoparticles. ACS. 2011, 27 (7): 4020-4028.Google Scholar
- Vaezi MR, Sadrnezhaad SK: Nanopowder synthesis of zinc oxide via solochemical processing. Mat Des. 2007, 28 (2): 515-519. 10.1016/j.matdes.2005.08.016.View ArticleGoogle Scholar
- Wang L, Muhammed M: Synthesis of zinc oxide nanoparticles with controlled morphology”. J Mater Chem. 1999, 9: 2871-2878. 10.1039/a907098b.View ArticleGoogle Scholar
- Yan C, Chen Z, Zhao X: Enhanced electroluminescence of ZnO nanocrystalline annealing from mesoporous precursors. Solid State Commun. 2006, 140 (1): 18-22. 10.1016/j.ssc.2006.07.030.View ArticleGoogle Scholar
- Pan A, Yu R, Xie S, Zhang Z, Jin C, Zou B: ZnO flowers made up of thin nanosheets and their optical properties. J Cryst Growth. 2005, 282 (1–2): 165-172.View ArticleGoogle Scholar
- Wu J-J, Liu S-C: Catalyst-Free Growth and Characterization of ZnO Nanorods. J Phys Chem B. 2002, 106 (37): 9546-9551. 10.1021/jp025969j.View ArticleGoogle Scholar
- Ghaffarian H, Saiedi M: “Synthesis of ZnO Nanoparticles by Spray Pyrolysis Method”. Iran J Chem Chem Eng. 2011, 30 (no. 1): 1-6.Google Scholar
- Zhang B, Ye X, Hou W, Zhao Y, Xie Y: Biomolecule-assisted synthesis and electrochemical hydrogen storage of Bi2S3 flowerlike patterns with well-aligned nanorods. J Phys Chem B. 2006, 110 (18): 8978-8985. 10.1021/jp060769j.View ArticleGoogle Scholar
- Zhang Y, Tian J, Li H, Wang L, Qin X, Asiri AM, Al-Youbi AO, Sun X: Biomolecule-assisted, environmentally friendly, one-pot synthesis of CuS/reduced graphene oxide nanocomposites with enhanced photocatalytic performance. ACS. 2012, 28 (35): 12893-12900.Google Scholar
- Wu S, Cao H, Yin S, Liu X, Zhang X: “Amino Acid-Assisted Hydrothermal Synthesis and Photocatalysis of SnO 2 Nanocrystals”. Phys Chem. 2009, 113: 17893-17898.Google Scholar
- Tong H, Zhu Y-J, Yang L-X, Li L, Zhang L, Chang J, An L-Q, Wang S-W: Self-Assembled ZnS Nanostructured Spheres: Controllable Crystal Phase and Morphology. J Phys Chem C. 2007, 111 (10): 3893-3900. 10.1021/jp066701l.View ArticleGoogle Scholar
- Fang KM, Wang ZZ, Zhang M, Wang AJ, Meng ZY, Feng JJ: Gelatin-assisted Hydrothermal Synthesis of Single Crystalline ZnO Nanostars and Their Photocatalytic Properties. J Colloid Interface Sci. Mar. 2013, Accepted manuscript (In press)Google Scholar
- Li Z, Xiong Y, Xie Y: Selected-control synthesis of ZnO nanowires and nanorods via a PEG-assisted route. Inorg Chem. 2003, 42 (24): 8105-8109. 10.1021/ic034029q.View ArticleGoogle Scholar
- Jha AK, Kumar V, Prasad K: Biosynthesis of Metal and Oxide Nanoparticles Using Orange Juice. Journal of Bionanoscience. 2011, 5 (2): 162-166. 10.1166/jbns.2011.1053.View ArticleGoogle Scholar
- Prakash T, Jayaprakash R, Sathya Raj D, Kumar S, Donato N, Spadaro D, Neri G: Sensing properties of ZnO nanoparticles synthesized by using albumen as a biotemplate for acetic acid monitoring in aqueous mixture. Sensors and Actuators B: Chemical. 2013, 176 (2010): 560-568.View ArticleGoogle Scholar
- Cai A-J, Wang Y-L, Xing S-T, Ma Z-C: Cavity of cyclodextrin, a useful tool for the morphological control of ZnO micro/nanostructures. Ceram Int . 2012, 38 (6): 5265-5270. 10.1016/j.ceramint.2012.03.037.View ArticleGoogle Scholar
- Qun Donga FK, Huilan S, Chunfu Z, Di Z, Qixin G: “Fabrication of hierarchical ZnO films with interwoven porous by a bioinspired templating technique.pdf”. Chem Eng J. 2008, 137: 428-435. 10.1016/j.cej.2007.05.045.View ArticleGoogle Scholar
- Han J, Su H, Xu J, Song W, Gu Y, Chen Y, Moon W-J, Zhang D: “Silk-mediated synthesis and modification of photoluminescent ZnO nanoparticles”. J Nanopart Res . 2012, 14 (no. 2): 726-View ArticleGoogle Scholar
- Tomczak MM, Gupta MK, Drummy LF, Rozenzhak SM, Naik RR: Morphological control and assembly of zinc oxide using a biotemplate. Acta Biomater. 2009, 5 (3): 876-882. 10.1016/j.actbio.2008.11.011.View ArticleGoogle Scholar
- Seeman NC: DNA in a material world. Nature. 2003, 421 (6921): 427-431. 10.1038/nature01406.View ArticleGoogle Scholar
- Gao X, Matsui H: Peptide-Based Nanotubes and Their Applications in Bionanotechnology. Adv Mater. 2005, 17 (17): 2037-2050. 10.1002/adma.200401849.View ArticleGoogle Scholar
- Hall SR, Bolger H, Mann S: “Morphosynthesis of complex inorganic forms using pollen grain templates Porous micron-sized particles of silica, calcium carbonate or by template-directed synthesis employing intact pollen”. Chem Commun. 2003, 44 (no. 0): 2784-2785.View ArticleGoogle Scholar
- Zhou H, Fan T, Zhang D: Hydrothermal synthesis of ZnO hollow spheres using spherobacterium as biotemplates. Micropor Mesopor Mat. 2007, 100 (1–3): 322-327.View ArticleGoogle Scholar
- Bin Hussein MZ, Yahaya AH, Ling PLC, Long CW: Acetobacter xylenium as a shape-directing agent for the formation of nano-, micro-sized zinc oxide. J Mater Sci. 2005, 40 (23): 6325-6328. 10.1007/s10853-005-3686-9.View ArticleGoogle Scholar
- Hussein MZ, Azmin WHWN, Mustafa M, Yahaya AH: Bacillus cereus as a biotemplating agent for the synthesis of zinc oxide with raspberry- and plate-like structures. J Inorg Biochem. 2009, 103 (8): 1145-1150. 10.1016/j.jinorgbio.2009.05.016.View ArticleGoogle Scholar
- Sotiropoulou S, Sierra-Sastre Y, Mark SS, Batt CA: “Biotemplated Nanostructured Materials †”. Chem Mater. 2008, 20 (no. 3): 821-834. 10.1021/cm702152a.View ArticleGoogle Scholar
- Myat M, Abdulkarim S: “Physicochemical and sensory characteristics of palm olein and peanut oil blends”. J Food. 2009, 7: 175-181.Google Scholar
- R. Submitted and P. Fulfillment: Fulfillment, Improvement Of Physico-Chemical Properties Of Palm Olein Blended With Rice Bran Oil By Surin Watanapoon. 2004,Google Scholar
- Zobir SAM, Abdullah S, Zainal Z, Sarijo SH, Rusop M: “Synthesis of carbon nano- and microspheres using palm olein as the carbon source”. Mater Lett. 2012, 78: 205-View ArticleGoogle Scholar
- Shahid EM, Jamal Y: Production of biodiesel: A technical review. Renew Sustain Energy Rev. 2011, 15 (9): 4732-4745. 10.1016/j.rser.2011.07.079.View ArticleGoogle Scholar
- Rudolph M, Erler J, Peuker UA: “A TGA–FTIR perspective of fatty acid adsorbed on magnetite nanoparticles–Decomposition steps and magnetite reduction. Colloids Surf A Physicochem Eng Asp. 2012, 397: 16-23.View ArticleGoogle Scholar
- Gyergyek S, Makovec D, Drofenik M: Colloidal stability of oleic- and ricinoleic-acid-coated magnetic nanoparticles in organic solvents. J Colloid Interface Sci. 2011, 354 (2): 498-505. 10.1016/j.jcis.2010.11.043.View ArticleGoogle Scholar
- Machunsky S, Grimm P, Schmid H-J, Peuker UA: “Liquid–liquid phase transfer of magnetite nanoparticles”. Colloids Surf A Physicochem Eng Asp. 2009, 348 (1–3): 186-190.View ArticleGoogle Scholar
- Mandal U: Ionic elastomer based on carboxylated nitrile rubber: infrared spectral analysis. Polymer international. 2000, 1657, no. July: 1653-1657.View ArticleGoogle Scholar
- Ramimoghadam D, Bin Hussein MZ, Taufiq-Yap YH: The Effect of Sodium Dodecyl Sulfate (SDS) and Cetyltrimethylammonium Bromide (CTAB) on the Properties of ZnO Synthesized by Hydrothermal Method. Int J Mol Sci. 2012, 13 (10): 13275-13293.View ArticleGoogle Scholar
- Ngamcharussrivichai C, Totarat P, Bunyakiat K: Ca and Zn mixed oxide as a heterogeneous base catalyst for transesterification of palm kernel oil. Appl Catal Gen. 2008, 341 (1–2): 77-85.View ArticleGoogle Scholar
- Rigby S, Fletcher R: “Experimental evidence for pore blocking as the mechanism for nitrogen sorption hysteresis in a mesoporous material”. J Phys Chem B. 2004, 15: 4690-4695.View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.